- Email: [email protected]

Ultrafast carrier capture in charged InAs quantum dots K.W. Sun *, A. Kechiantz

1

Department of Applied Chemistry and Institute of Molecular Science, National Chiao Tung University, 1001 Da Hseuh Road, Hsinchu, Taiwan Available online 16 May 2006

Abstract We report theoretical and experimental results of our investigation on carrier capture and relaxation processes in undoped and modulation-doped InAs/GaAs self-assembled quantum dots (QDs). We ﬁnd that carrier capture and relaxation in the ground state is faster in the modulation-doped quantum dots compared to the case in neutral dots at an excitation level as low as one electron–hole pair per dot. The ultrafast photoluminescence (PL) transient rise time observed in the charged dots is attributed to the relaxing of strained ﬁeld induced by the presence of cold carriers in the dots. The Hamiltonian of electron’s interaction with local vibrating ﬁeld and carrier capture time are also calculated. 2006 Elsevier B.V. All rights reserved. PACS: 61.46.+w; 78.47.+p; 78.55.m Keywords: Laser–matter interactions; Optical spectroscopy; Quantum wells, wires and dots; Luminescence; Ultrafast processes and measurements; Upconversion; Time resolved measurements

1. Introduction Quantum dots (QDs) are the subject of a rapidly developing area in semiconductor research. Many groups have reported the fabrication of InAs on GaAs by methods of self-organized growth. One of the prominent fabrication methods for QDs is the Stranski–Krastanov (S–K) process which uses the lattice mismatch between the substrate and the over layers [1–3]. Formation of ordered pyramidalshaped QDs was observed on a residual two-dimensional layer above a nominal coverage of two monolayer (ML) for InAs on GaAs (0 0 1) substrates by Ruvimov and coworkers [4]. Segregation of InAs wetting layers (WLs) was investigated by Oﬀermans et al. using cross-section scanning tunneling microscopy [5]. It was concluded that the formation of WLs is a delicate interplay between sur*

Corresponding author. Tel.: +886 3 5712121x56582; fax: +886 3 572 3764. E-mail address: [email protected] (K.W. Sun). 1 Address: Scientiﬁc Research Division, State Engineering University of Armenia, Yerevan, Armenia. 0022-3093/$ - see front matter 2006 Elsevier B.V. All rights reserved. doi:10.1016/j.jnoncrysol.2006.03.015

face migration, strain-driven segregation, and the dissolution of QDs during growth. Calculations also indicated that the WL considerably aﬀects both the single-particle energy and wave function [6]. Recently, a new self-organized growth method using droplet epitaxy was reported for direct formation of QD systems without WLs [7,8]. The study of carrier relaxation and capture in InAs/ GaAs QDs [9–12] has attracted much attention due to their unique optical and electrical properties for potential device applications. It has been shown that the removal of WL does not aﬀect the carrier capture and relaxation in QDs [13]. Recently, Yuan et al. [14,15] studied the carrier dynamics in InAs/GaAs QDs. Their observation on systematically longer PL risetimes in the higher excited states was interpreted in the frame work of sequential state ﬁlling, resulting from fast trapping and intra-dot relaxation. However, few experiments have examined carrier dynamics in charged QDs. In a recent work done by Gu¨ndog˘du et al. [16,17], carrier capture and relaxation to the ground state was found to be much faster in the highly charged dots compared to the neutral dots. Their results for p-doped QDs reveal a threefold decrease in the room temperature electron capture and

2356

K.W. Sun, A. Kechiantz / Journal of Non-Crystalline Solids 352 (2006) 2355–2359

relaxation time relative to corresponding undoped QDs. The enhancement of carrier capture and relaxation was attributed to the rapid electron–hole scattering involving the built-in carrier population. In this paper, we investigate the carrier capture and relaxation process in undoped, lightly n-doped and pdoped InAs/GaAs QDs using time-resolved luminescence up-conversion spectroscopy techniques. We report observation of ultrafast carrier capture and relaxation in the charged QDs’ ground states at very low doping concentrations and at low excitation levels. We have proposed a model for interpreting our experimental results. A comparison between experiments and calculations allows us to conclude that the presence of the few cold carriers has a signiﬁcant inﬂuence on the capture and relaxation in the charged QDs. 2. Experiments and results The InAs QD samples were grown by using a solid source molecular beam epitaxy (MBE) machine [18]. The growth procedure and condition are described as follows. After native oxide desorpted under As ﬂux at 610 C, a ˚ GaAs buﬀer layer was deposited at 570 C to 2500 A ˚ Al0.3Ga0.7As and recover the substrate surface. 300 A ˚ GaAs were deposited at a growth rate of 1 lm/h 1400 A ˚ GaAs was grown at the same temperature. Then, 100 A at a growth rate of 0.3 lm/h. In the meanwhile, the substrate temperature is lowered down (520 C) for InAs deposition, and the desired As ﬂux for QDs growth was achieved by adjusting the needle valve of the As cracker cell. Afterwards, 10 nm GaAs capped layer was deposited at the same temperature of QDs growth with a growth rate of 1 lm/h. Then the substrate temperature and As ﬂux were raised to the original values for GaAs and Al0.3Ga0.7As growth. Finally, a layer of uncapped QDs was grown with the same conditions, and then the substrate cooled down under As ﬂux immediately. The n-doped (p-doped) samples contain a Si-delta (Be-delta) doping layer 2 nm below the QD layer with nominal densities of about 2 · 1010 cm2. The average sheet density of the QDs is about 2 · 1010 cm2. Images from atomic force microscopy (AFM) measurements reveal circular shaped QDs with an average dot size of approximately 20 nm in base width and a height of about 5 nm. Free carriers from the doped layer accumulated in the low energy states within the InAs QDs. In the lightly doped samples, most of the dots only contain a single electron or hole. The measurements of carrier dynamics were performed by time-resolved photoluminescence with time-resolution of about 200 fs. The self-mode-locked Ti:sapphire laser was operated at 788 nm with spectral width of about 18 meV (full width at half maximum) to excited carriers in the GaAs barrier. According to the focus spot size and the absorption depth at the photoexcitation wavelength, the laser pumping power was adjusted to give injected carrier densities from 2 · 1010 cm2 (low) to 5 · 1011 cm2

(high), respectively. The accuracy of the excitation density is approximately a factor of two. The room temperature steady state PL spectra of the undoped QD sample taken at an excitation wavelength of 788 nm and intensity of 1 · 103 W/cm2 are shown in Fig. 1. The spectral lines centered at 872 nm and 930 nm are attributed to the bandgap energies of the GaAs and WLs (as shown in Fig. 1(a)), respectively. Three spectrally well-separated PL lines n = 1 (ground state), n = 2 and n = 3 (excited states) at longer wavelengths (as shown in Fig. 1(b)) are due to electron–hole recombination between distinct QD states of the conduction and valence bands. Only the n = 1 peak is observed at low excitation intensity and it is assigned as the QD ground electron to ground hole transition. The center wavelengths of the spectral peak n = 1 to n = 3 are 1235 nm, 1160 nm and 1085 nm, respectively. The energy separations (also shown in Fig. 1(b)) between the QD conﬁned states are 65 and 74 meV. In the PL studies on modulation-doped QDs, due to the lightly doping, we did not observe signiﬁcant changes in the spectra lineshape or shift-

Fig. 1. Room temperature PL spectra of InAs/GaAs self-assembled QDs, displaying GaAs barrier, wetting layer and excited state radiative recombination in wavelength range from (a) 820 to 950 nm and (b) 950 to 1300 nm. Spectra were excited at 788 nm with a self-mode-locked Ti:sapphire laser.

K.W. Sun, A. Kechiantz / Journal of Non-Crystalline Solids 352 (2006) 2355–2359

2357

ing of ground-state optical transition. Carrier capture and relaxation to the QD’s ground level are examined as a function of excitation density and temperature by measuring PL rise times at the energy of QD ground state identiﬁed in the steady state PL spectra. The time evolution of the PL signal then follows from the analysis of the rate equations IðtÞ / A ½expðt=sr Þ expðt=sd Þ=ðsr sd Þ; where sr and sd are the PL rise and decay time constants, respectively. In Fig. 2 we show PL transients detected at the ground state of the undoped QDs for the ﬁrst 20 ps at low temperature. Time-resolved PL measured at the same energy but at three diﬀerent excitation levels (low, moderate and high) is displayed in parallel for comparison. The PL rise times of the ground state in the QDs accelerate as the excitation power increases and reach a value of less than 1 ps at a photoexcited carrier density P1 · 1011 cm2. It is believed that the carrier density dependence of the ultrafast relaxation is due to Auger-like carrier–carrier scattering [9]. Experiments on our modulation-doped QDs allow the relaxation dynamics of electrons and holes to be investigated separately. At low temperature, low excitation densities, the photo-generated carriers do not signiﬁcantly perturb the well-deﬁned Fermi distribution of doped cold carriers. Therefore, the luminescence dynamics is dominated by the electron (hole) dynamics in p (n) modulation-doped QDs. For the modulation-doped samples with doping density of only 2 · 1010 cm2, only the lowest electron (n-doped QDs) or hole (p-doped QDs) level is occupied prior to the optical excitation. The initial transient

Fig. 2. Time-resolved photoluminescence intensity measured at the energy of the undoped QDs’ ground states at three diﬀerent excitation levels and at low temperature. The solid curves indicate ﬁts of the PL rise to a single exponential.

Fig. 3. Results of time-resolved PL experiments at 77 K for p-doped (circles), n-doped (squares) and undoped QDs (triangles).

PL at the ground-state optical transition in the modulation-doped QDs at low temperature is shown in Fig. 3. The results in Fig. 3 correspond to an optical excitation level of only one electron–hole pair per dot. Therefore, the major diﬀerence between the time-resolved PL experiments on the charged and uncharged QDs is the presence of small built-in electron (hole) population in the n-doped (p-doped) QDs prior to optical excitation. However, the ﬁts of the PL transients in Fig. 3 indicate capture times of less then 2 ps for charged QDs which are more rapid than in the undoped QDs, regardless of the species of cold carrier involved. The time-resolved PL rise times also show no discernible temperature dependence for both the charged and uncharged QDs. In contrast to the earlier report on carrier capture and relaxation in highly charged QDs [16,17], the total carrier densities in our experiments are only on the order of 2 · 1010 cm2. According to the results reported in Ref. [19], for a plasma density of 1010 cm2 and a quantum dot lateral size of 20 nm, the calculated Auger scattering rate was only on the order of 2 · 1010 s1. Therefore, it is unlikely that the Coulomb scattering within the electron–hole plasma is responsible for the ultrafast carrier capture and relaxation observed in our charged QD experiments. The observation of no discernible temperature dependence on the PL transient rise time also indicates that phonon scattering was not responsible for the accelerated carrier capture observed in our experiments. In the following section, a theoretical model is proposed to interpret our experimental results. 3. Theoretical model We model a circular shaped InAs QD with a base diameter of 20 nm and a height of 2 nm. In response to

2358

K.W. Sun, A. Kechiantz / Journal of Non-Crystalline Solids 352 (2006) 2355–2359

the localized (doped) charges in the dots, a polarization ~R V ð~ ﬁeld ~ P ð~ RÞ ¼ e0 r RÞ (where V ð~ RÞ ¼ eð1 1=es Þ=4pe0 R and es is the static dielectric constant of semiconductor) must be induced around the QDs. During the scattering, electron (or hole) must encounter two electric ﬁelds of opposite signs. Those ﬁelds are positive (negative) ﬁeld of a bare hole (electron) conﬁned within the dot and screening ﬁeld of local polarizations around the dot. When the electric ﬁeld inducing the strain around the dots suddenly disappears due to the capture of an electron or a hole into the QDs, local strain of crystal lattice must trigger vibrations of ions and bond electrons around the dot to relax the strain and to release the energy. When a mobile electron was scattered on the polarization ﬁeld produced by positively charged dots, by Fourier transforming this polarization ﬁeld, the electron energy in the polarization ﬁeld Ekc can be expressed by the sum of partial contributions from local strains with wave number q, Z e2 ð1 1=es Þ sinðqRÞ dq: ð1Þ Eev ¼ 2p2 e0 qR Assuming that the system of ions and bond electrons is linear during interaction, the decay of locally induced vibrations is given by the Bessel function J0(xmt), where xm is the maximum value of phonon frequency [20]. For simplicity we assume that polarization induces constant potential, V(R0), within the dot, i.e. the volume of the dot is never polarized, where R0 is the average radius of quantum dot. Then for electron interacting with local vibrations triggered within the dot at the time t0, the time-dependent Hamiltonian can be written as Z e2 ð1 1=es Þ sinðqR0 Þ H ev ðt t0 Þ ¼ J 0 ½xm ðt t0 Þ 2p2 e0 qR0 ð2Þ qR0 ð1 R=R0 Þdq; where qR0(1 R/R0)/xm is the time that vibration with wave number q takes to arrive to a point R within the dot. The Hamiltonian Hev(t t0) brings short-time perturbation to the electron scattering processes and it can result in the capture of photoexcited carriers into the QD’s conﬁned states. Due to low photoexcitation densities, number of excitons created in the sample was no more than one exciton per dot. Distance between QDs was far enough so that the Coulomb interaction was negligible. Therefore, the Coulomb interaction was not included in the Hamiltonian. Denote n the density of mobile electrons and X the volume of quantum dot. In the frame of time-dependant perturbation theory, if the wave function of mobile states jki is normalizedR to the ﬂow of onepﬃﬃﬃﬃﬃﬃ electron per second, the 2 rate W ¼ j hcjH ev ðt t0 Þjkidtj nX= h2 Dt of the variationassisted transitions of electrons from mobile into conﬁned electronic state jci can be written as W ¼

e4 ð1 1=es Þ2 n1=2 1=6 16p2 e20 h 2 x m R0

2

F ðDtÞjKðkÞj ;

ð3Þ

where Z 2 xm Dt ; J ðx tÞ exp½x tdt ð4Þ 0 m kc Dt 0 Z Z ð12=pÞ1=4 sinðqR0 Þ exp½i~ k~ R KðkÞ ¼ 3=2 q p R0 xkc qR0 ð1 rÞ exp i qð1 rÞ B Dt wc dq dR3 ; xm xm

F ðDtÞ ¼

ð5Þ and B½v ¼

Z

v

J 0 ðxm zÞ expðixkc zÞdz

Z

0

Dt

J 0 ðxm zÞ exp½ixkc zdz:

0

ð6Þ Here ~ k is the electron wave vector in mobile state, wc is the electron wave function in conﬁned state, hxkc is the energy separation between conﬁned and mobile electronic states in quantum dot and r = R/R0. Vibrations around the quantum dot decay as cylindrical Bessel function J0(xmt). By approximating the conﬁned electronic states with pﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃ the spherical Bessel function, Wc ¼ 2=3p j0 ðp rÞ= X, Eq. (5) can be further reduced to KðkÞ ¼

pﬃﬃﬃ Z 4 4 3 xm Dt sin qR0 dq p3=4 0 q Z 1 ixkc qR0 ð1 rÞ sinðkR0 rÞ dr exp : sinðrpÞ x kR0 m 0 ð7Þ

Therefore, the rate of carrier capture into the QDs s = 1/W is calculated to be 5=2

s¼

16p2 e20 hm ðx2kc x2m ÞR0 e4 ð1 1=es

Þ2 n1=2 jKðkÞj2

:

ð8Þ

Fig. 4. Dependence of oscillation frequency F(Dt) on xmDt (dash curve) xm for xkc/xm = 4.286. When xmDt > 1, F(Dt) can be reduced to ðx2 x 2 ÞDt m kc (solid line) for xkc/xm = 4.286.

K.W. Sun, A. Kechiantz / Journal of Non-Crystalline Solids 352 (2006) 2355–2359

The rate s is mainly decided by the energy separation of conﬁned states hxkc, the duration of perturbation Dt and the function F(Dt). The dependence of F(Dt) on xmDt is plotted in Fig. 4 for InAs/GaAs quantum dots with hxkc = 150 meV and hxm = 36 meV. For the given parameters in our p-doped QD experiments, Eq. (8) gives a capture rate of s = 1.7 ps. This calculated value is in good agreement with our experimental results. In the case of holes been captured in an n-doped QD, the calculations should taking into account the warping of valence bands due to the quantum conﬁnement and strain. 4. Conclusion In conclusion, we have investigated carrier capture and relaxation in the ground state of undoped and modulation-doped InAs/GaAs QDs. We observe faster capture and relaxation processes in the charged QDs in comparing to the undoped dots even in the one electron–hole pair per dot regime. Our results suggest that, under low excitation intensity and low doping level, the relaxing of polarization ﬁeld induced by the conﬁned charge in the quantum dot is the dominant factor for the acceleration of carrier capture. Our calculations also show that carriers interact with decaying ﬁeld results in ultrafast capture into conﬁned electronic states. We have performed calculations reproducing the experimental conditions used in our experiments and a capture time of 1.7 ps was obtained from our calculations. Acknowledgement This work was supported by the National Science Council of Republic of China under contract No. NSC 93-2112M-259-009.

2359

References [1] R. No¨tzel, J. Temmyo, T. Tamanura, Nature 12 (1994) 131. [2] K. Nishi, T. Anan, A. Gomyo, S. Kohmoto, S. Sugou, Appl. Phys. Lett. 70 (1997) 3579. [3] V. Bressler-Hill, S. varma, A. Lorke, B.Z. Nosho, P.M. Petrov, W.H. Weinberg, Phys. Rev. Lett. 74 (1995) 3209. [4] S. Ruvimov, P. Werner, K. Scheerschmidt, U. Go¨sele, J. Heydenreich, U. Richter, N.N. Ledentsov, M. Grundmann, D. Bimberg, V.M. Ustinov, A.Yu. Egorov, P.S. Kop’ev, Zh.I. Alferov, Phys. Rev. B 51 (1995) 14766. [5] P. Oﬀermans, P.M. Koenraad, R. No¨tzel, J.H. Wolter, K. Pierz, Appl. Phys. Lett. 87 (2005) 111903. [6] S. Lee, O.L. Lazarenkova, P. von Allmen, F. Oyafuso, G. Klimeck, Phys. Rev. B 70 (2004) 125307. [7] C.-D. Lee, C. Park, H.J. Lee, K.-S. Lee, S.-J. Park, C.G. Part, S.K. Noh, N. Koguchi, Jpn. J. Appl. Phys. 37 (1998) 7158. [8] T. Mano, K. Watanabe, S. Tsukamoto, H. Fujioka, M. Oshima, N. Koguchi, Jpn. J. Appl. Phys. 38 (1999) L 1009. [9] J.Y. Marzin, J.M. Gerald, A. Izael, D. Barrier, G. Bastard, Phys. Rev. Lett. 73 (1994) 716. [10] D. Leonard, M. Krisgnamurthy, C.M. Reaves, S.P. Densaars, P.M. Petrov, Appl. Phys. Lett. 63 (1993) 3203. [11] U. Bockelmann, G. Bastard, Phys. Rev. B 42 (1990) 8947. [12] H. Benisty, C.M. Sotomayor Torres, C. Weisbuch, Phys. Rev. B 44 (1991) 10945. [13] S. Sanguinetti, K. Watanabe, T. Tateno, M. Wakaki, N. Koguchi, T. Kuroda, F. Minami, M. Gurioli, Appl. Phys. Lett. 81 (2002) 613. [14] Z.L. Yuan, E.R.A.D. Foo, J.F. Ryan, D.J. Mowbray, M.S. Skolnick, M. Hopkinson, Physica B 272 (1999) 12. [15] Z.L. Yuan, E.R.A.D. Foo, J.F. Ryan, D.J. Mowbray, M.S. Skolnick, M. Hopkinson, Phys. Status Solidi (b) 224 (2001) 409. [16] K. Gu¨ndog˘du, K.C. Hall, Thomas F. Boggess, D.G. Deppe, O.B. Shchekin, Appl. Phys. Lett. 84 (2004) 2793. [17] K. Gu¨ndog˘du, K.C. Hall, Thomas F. Boggess, D.G. Deppe, O.B. Shchekin, Appl. Phys. Lett. 85 (2004) 4570. [18] L. Chu, A. Arzberger, G. Bo¨hm, G. Abstreiter, J. Appl. Phys. 85 (1999) 2355. [19] U. Bockelmannand, T. Egeler, Phys. Rev. B 46 (1992) 15574. [20] P. Taylor, O. Heinonen, A Quantum Approach to Condense Matter Physics, University Press, Cambridge, 2002.

Copyright © 2021 COEK.INFO. All rights reserved.